- Home
- Documents
*Quantum and Classical Magnetoresistance in and Classical Magnetoresistance in Ambipolar Topological*

prev

next

out of 12

View

212Download

0

Embed Size (px)

1

Supplemental Materials

Quantum and Classical Magnetoresistance in Ambipolar Topological Insulator Transistors with Gate-tunable Bulk and Surface Conduction

Jifa Tian1,2,*, Cuizu Chang3,4, Helin Cao1,2, Ke He3, Xucun Ma3, Qikun Xue4 and Yong P. Chen1,2,5,#

1. Department of Physics, Purdue University, West Lafayette, Indiana 47907, USA

2. Birck Nanotechnology Center, Purdue University, West Lafayette, Indiana 47907, USA

3. Beijing National Laboratory for Condensed Matter Physics, Institute of Physics, Chinese Academy of Sciences,

Beijing 100190, P. R. China

4. State Key Laboratory for Low-Dimensional Quantum Physics, Department of Physics, Tsinghua University,

Beijing 100084, P. R. China

5. School of Electrical and Computer Engineering, Purdue University, West Lafayette, Indiana 47907, USA

*Email: tian5@purdue.edu; #Email: yongchen@purdue.edu

2

Figure S1 Sheet resistance at zero B-field measured as a function of temperature (T) with Vg=10 V

(duplicated from Fig. 1c). We have fitted our experimental data (red solid line) below 55 K to a simple

model (back dashed line is the fitting result) similar to that developed in Ref. S1 to estimate the surface to

bulk conductance ratio. This model assumes the total conductance Gt consists of two parallel channels: a

thermally activated bulk with conductance Gb, and a metallic conduction (GS) which we attribute to the

surface. At low T, the bulk conduction freezes out, and the residual metallic surface conduction dominates.

More specifically, we fit the measured Gt(T) to , with 1/ and 1/ , where represents a bulk activation gap between the Fermi level and the edge of

the bulk band, A accounts for the static disorder scattering and B represents electron-phonon scattering

affecting the surface carriers (Ref. S1). The fit of the data yields =200 K, Rb0=246.3 /, A=4100 /,

and B=1.68 /(K). Based on these values, one obtains Rb(T=20 K)=193 k/ and RS(T=20 K)=4.1

k/, giving a surface to bulk conductance ratio of GS/Gb=Rb/RS~50 at T=20 K, suggesting the surface

conduction will dominate the charge transport at low temperature (GS/Gb>50 for T

3

maximum) is relatively small compared to the bulk band gap, consistent with the DP expected to be

located relatively close to the valence band edge [S3] (in addition, the spatial charge inhomogeneity and

mismatched top and bottom surface DP positions can further reduce the activation energy).

Figure S2 Color plots of the magnetoresistance Rxx=Rxx(B)-Rxx(B=0T) vs B and Vg at two different

temperatures: (a) 3D color surface plot and (b) 2D color plot for T=2.8 K; (c) 3D color surface plot and (d)

2D color plot for T=25 K.

4

Figure S3 A zoomed in view of the upper panel of Fig. 2c showing the magnetoresistance Rxx=Rxx(B)-

Rxx(B=0T) vs B for different Vg at T=25 K, where LMR becomes prominent and starts from very low B

(

5

Figure S4 The extracted gate capacitance C per unit area (from Fig. 3c) and effective relative dielectric

constant r of the 250 m-thick STO substrate vs T.

6

Figure S5 The gate dependence of the carrier density n extracted using a 1-band model from Fig. 2a at

T=1.4 K. For Vg far away from CNP (~40 V), Rxy(B) is linear (Fig. 2a) and n has a linear dependence on

Vg. As Vg is close to CNP for both n-type and p-type regimes, Rxy(B) becomes nonlinear (Fig. 2a) due to

multiple-band transport (eg., coexistence of electron and hole carriers), the n (extracted from 1-band

model using the low-B slope of Rxy) deviates from the linear Vg dependence and its magnitude provides an

upper bound for the actual net carrier density [S2]. The dashed line indicates the expected general trend of

one-band-extracted n vs Vg as the system goes through the ambipolar transition [S2]. Inset is the zoom-in

of n vs Vg near the CNP. We estimate the maximum surface carrier (hole) density achieved when the

Fermi level (Ef) is at the top of BVB to be n~1.21013 cm-2, for two surfaces combined), using n=kF2/2,

where kF is the Fermi wavevector based on the ARPES measured band structure (near BVB) in Ref. S3. It

is expected that the Dirac point of the TSS is closer to the BVB than to the bulk conduction band (BCB,

Ref. S3, even though the detailed band structure near the bottom of BCB has not been measured),

suggesting that the maximum carrier (electron) density that can be accommodated by two surfaces (when

Ef is at the bottom of BCB) is even larger than ~1.21013 cm-2.

7

Figure S6 Representative sheet conductance (G=G(B)-G(B=0T)) as a function of B field, for (a) Vg=-

10 V and (b) Vg=44 V, both measured at T=1.4 K. Each red curve is the fit using the HLN model (Eq. 1)

in the low-B regime (up to 2 T) and green dotted line is the linear fitting of the LMR at high-B regime

(from 2 T to 6 T).

Figure S7 Estimated gate-dependent (a) mean free path l, (b) diffusion constant D, and phase coherence

time for surface state carriers, at different temperatures. The mean free path l is estimated from

l=h/(e2kF) with Fermi wave vector 2 using measured zero-B-field 2D electrical conductivity (=G) and 1-band total Hall density n; diffusion constant D from =v with v =4105 m/s (based on ARPES measurement value [S3]), and phase coherence time using = /D (with L from Fig. 4c). We

note that for Vg

8

Figure S8 The slope k of LMR vs np (of one-band p-type carriers mostly from BVB) at different

temperatures, demonstrating the LMR is significantly enhanced as Ef approaches TSS.

9

Figure S9 (a) The =Rxx(6T)-Rxx(3T) vs Vg at different temperatures, demonstrating the LMR is

significantly enhanced as Ef approaches TSS; (b) vs T at five representative gate voltages; (c)

vs np (for one-band p-type carriers mostly from BVB, same np data points as in Fig. 3c) at different

temperatures. We find that cannot be fitted to a single power law (either 1/np2 (Abrikosov) or 1/np

(Wang-Lei)) over this density range, but rather appear to cross over from a ~1/np behavior (indicated by

the pink band) for np>41013 cm-2 to ~1/np2 behavior (purple band) for np

10

Figure S10 The slope k of LMR vs mobility (for one-band p-type carriers mostly from BVB) at

different temperatures. When is smaller than ~100 cm2/Vs, k is approximately proportional to , while k

rise sharply and becomes less well correlated with when approaches ~100-130 cm2/Vs (highlighted

by the grey band). We note this threshold mobility is close to the maximum 0 fitted in the vs. np

dependence (inset of Fig. 3d).

11

Figure S11 (a) The crossover field BC as a function of carrier mobility ; (b) 1/BC as functions of ; (c)

the crossover field BC on left axis and Hall mobility on right axis as a function of Vg at various

temperatures. The crossover field BC (obtained from the first-order derivative of the MR curve versus B

field) is the field at which the MR curve changes from parabolic to linear (i.e., MR derivative approaching

a constant). The data points involve only include those for one-band p-type carriers.

12

Figure S12 The 1/BC as a function of the slope k of LMR at various temperatures for all gate voltage

values measured.

References:

S1 Gao, B. F., Gehring, P., Burghard, M., Kern, K. Gate-controlled linear magnetoresistance in thin

Bi2Se3 sheets. Appl. Phys. Lett. 100, 212402 (2012).

S2 Hong, S. S., Cha, J. J., Kong, D. & Cui, Y. Ultra-low carrier concentration and surface-dominant

transport in antimony-doped Bi2Se3 topological insulator nanoribbons. Nat. Commun. 3, 757 (2012).

S3 Zhang, J. et al. Band structure engineering in (Bi1xSbx)2Te3 ternary topological insulators. Nat.

Commun. 2, 574 (2011).